BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS

 Patrick Perkins
 6 months ago
 Views:
Transcription
1 BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency , Ohsawa, Mitaka, Tokyo, JAPAN ABSTRACT In this study, biaxial failure strength of quasiisotropic CFRP (carbon fiber reinforced plastic) composite laminate was investigated experimentally. Inplane biaxial tests with using CFRP cruciform specimens were conducted to measure biaxial failure strains with strain gauges. High speed photographs of biaxial fracture indicated that failure in the cruciform specimen was initiated at gauge area and breakage was developed to GFRP (glass fiber reinforced plastic) tab regions of the specimen. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with strip specimens. Both failure strains were approximately coincident, which proved the validity of the inplane biaxial strength tests with cruciform specimens. Failure strain in the direction of higher load was approximately constant in the first quadrant of failure envelope. Failure strain under uniaxial tensile stress was higher than those under biaxial tensile stress. Keywords: CFRP laminate, Biaxial load, Cruciform Specimen, Failure Envelope, Biaxial Strength INTRODUCTION New engineering materials are being developed to improve performance for vehicle structures. Especially, light weight and high strength materials are expected in aeronautical, astronautical and transportation industries. Applications of composite materials, as light weight materials, are recently widening for aerospace structures. Multiaxial failure criteria of the composite materials are very important for design of the aerospace structures, but have been not yet sufficiently established due to microscopic anisotropy and complicated fracture mechanisms in the composite materials. Many damage and failure criteria for composite materials under multiaxial stresses have been proposed and evaluated using experimental data [1]. Substantial experimental data is needed to assess the prediction by the proposed criteria. However, multiaxial strength data is not enough for new materials because multiaxial testing methods do not become widely used due to difficulties to conduct tests and particularity of facilities. Many methods to evaluate the multiaxial mechanical characteristics are suggested. One of the effective methods to acquire the biaxial mechanical properties of the plate is an inplane biaxial testing with a planar cruciform specimen.
2 Inplane biaxial tests with cruciform specimens had been employed to measure the biaxial mechanical properties of fabrics and yield locus of metal materials for decades. Recently biaxial mechanical properties of composite materials were obtained with using cruciform specimens. Mailly et al.[2] measured biaxial strength of GFRP unidirectional materials with cruciform specimens. They reported substantial influence of longitudinal stress on transverse nonlinearity of GFRP materials. Smits et al.[3] investigated effect of cruciform specimen geometries on biaxial failure strain of GFRP laminates, and determined a suitable geometry for biaxial testing of fiber reinforced composites. Welsh et al.[4] experimentally acquired twodimensional failure envelope for quasiisotropic CFRP laminates with using cruciform specimens, and estimated failure stress with φ R φ160 φ [unit:mm] Fig.1. CFRP cruciform specimen. Fig.2. Biaxial Testing Machine. Fig. 3. Finite element mesh of quarter model of cruciform specimen. Table 1. Elastic constants of HTA/#101 CF/epoxy quasiisotropic laminate. Property E(GPa) 49.4 G(GPa) 18.9 ν 0.31 Table 2. Elastic constants of GFRP laminate. Property E(GPa) 30.0 G(GPa) 11.5 ν 0.3
3 bypass correction factor. In Japan Aerospace Exploration Agency(former National Aerospace Laboratory of Japan), Susuki[5] conducted biaxial fatigue tests with cruciform specimens for fiber reinforced composites in addition to static fracture tests, and the results indicated that biaxial loading phase has significant impact on fatigue strength of the composite laminates. Khamsesh et al.[6] carried out openhole biaxial compression tests for CFRP composite laminates, and identified failure mechanisms of composite laminate with openhole under biaxial compressive load. In this study, biaxial strength of quasiisotropic CFRP composite laminates was experimentally acquired. Inplane biaxial tests with using CFRP cruciform specimens were conducted to measure biaxial failure strains with strain gauges. Strain and stress distributions in gauge area of the cruciform specimen were evaluated by finite element analysis and compared to validate measured strain level and ratio. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with strip specimens to prove the validity of the inplane biaxial strength tests. Influence of biaxial loadings on failure strains of quasiisotropic CFRP laminates were evaluated by the experimental results. EXPERIMENTAL PROCEDURE Cruciform Specimen Material used in this study was carbon fiber/180 C cured epoxy HTA/#101. Stacking sequence of specimens was (0/90/45/45)s. Thickness of the laminates was about 1.0mm. GFRP tabs are bonded on both sides of the CFRP laminate. Geometry of the biaxial cruciform specimens is shown in Fig. 1. The cruciform specimen geometry was determined based on specimens that Susuki proposed in [5]. The cruciform specimen was designed to apply the biaxial load with pin connections between four arms of the cruciform specimen and cross heads of a biaxial testing machine. However, applying load to the specimen with the pin connections was insufficient to achieve the final failure. Then hydraulic wedge grips were employed to connect the arms of the cruciform specimen to the cross heads of the biaxial testing machine in this study. InPlane Biaxial Testing Machine The biaxial testing machine used in this study consists of four hydraulic actuators of 245kN (tension/compression) capacity for static load. These four actuatorassemblies are diagonally mounted in an octagonal boxshaped frame (Fig. 2). Each loading axis is depicted as x and yaxis. The testing machine can apply biaxial load with arbitrary load ratio to a cruciform specimen. One advantageous aspect of inplane biaxial tests with cruciform specimens is that biaxial strain or stress ratio can be set arbitrarily. A particular problem with the operation of cruciform type biaxial test has been controlling to minimize the drift of the specimen center with load control. A small rigid movement during the biaxial test can give undesirable side force and unexpected damage to the cruciform specimen. It seems to be difficult to control four actuators not to generate imbalance at all by load feedback signals only. A double loop feedback control system was developed to carry out static tests and fatigue tests without readjustments of the specimen position.
4 Because of the round shaped reinforcement of GFRP tabs around the gauge area, stresses in the center portion of the specimen are not simply predictable. Before biaxial strength tests, the strains induced by the biaxial loads in the gauge area are needed to be obtained as functions of biaxial load. The relationships between biaxial loads and strains are used to determine biaxial load ratio to achieve prescribed biaxial strain (or stress) ratio. FINITE ELEMENT ANALYSIS Strain and stress distributions in the gauge area of the cruciform specimen were evaluated with using ABAQUS 6.71, a commercial software package for finite element analysis developed by SIMULIA. The elastic constants of carbon fiber/180 C cured epoxy HTA/#101 quasiisotropic laminate and GFRP laminate used in the numerical analysis are shown in Tables 1 and 2, respectively. The symbols E, G, ν in these tables refer to extensional modulus, shear modulus and Poisson s ratio, respectively. The calculations for the cruciform specimen under biaxial loadings were conducted under the assumptions of linearelastic and nondamage development with 1/4 model as shown in Fig. 3. The finite element model consists of 8node brick elements. It is assumed for simplicity that there are no holes in the arms of the cruciform specimen and biaxial load was applied to arm ends of the cruciform specimen directly. In this study, x and y axes coincide with the 0º and 90º directions of laminates respectively, and the z axis is the direction through the ply thickness. RESULTS AND DISCUSSIONS Calculated Strain and Stress Distributions Numerically calculated stress and strain distributions in the CFRP cruciform specimen under uniaxial loading F x =100kN, F y =0kN (F x : F y =1:0) are shown in Fig. 4, where F x and F y mean x and ydirectional applied forces, respectively. Xdirectional stress and strain in the gauge area are higher than other regions as shown in Fig. 4(a) and (b), respectively. Ydirectional stress in the gauge area in Fig. 4(c) was compressive when the specimen is subjected to xdirectional uniaxial tensile load. Ratio of ydirectional contraction in Fig. 4(d) to xdirectional extension in Fig. 4(b) is higher than Poisson's ratio due to the transverse compression. It is noted that stress field is not uniaxial stress state in the gauge area of the cruciform specimen, even though the cruciform specimen is subjected to uniaxial load. Calculated stress and stress distributions in the CFRP laminate under biaxial loading F x = F y =100kN (F x : F y =1:1) are shown in Fig. 5. Stress and strain distributions in case of F x = F y are symmetrical about the line x=y because the cruciform specimen geometry, the stacking sequence and the applied biaxial load are symmetric. Biaxial stress and strain ratios in the gauge area are also 1:1 when the specimen is subjected to biaxial load with load ratio F x : F y =1:1. Maximum normal stress and strain in the gauge area in Fig.5(F x : F y =1:1) are less than those in Fig. 4(F x : F y =1:0) due to Poisson s ratio and round shaped reinforcement of GFRP tabs. Numerical and experimental results of biaxial strains under uniaxial and biaxial loading (F x : F y =1:0 and 1:1) in the strain range within 0.3% are compared in Fig. 6. These
5 figures show that numerical results are in good agreement with experimental results, and biaxial strain ratio changes in relation to the biaxial loading ratio. Relationships among Biaxial Load, Strain and Stress Relationships among xdirectional uniaxial load F x, strains (ε x and ε y ) and stresses (σ x and σ y ) in the strain range within 0.3% are shown in Fig. 7, where ε i and σ i (i=x, y) are idirectional normal strain and stress, respectively. Strains (ε x and ε y ) were measured by using strain gauges. Stress in the gauge area can be calculated from cross sectional area in the gauge area and force that carried through the gauge area conceptually. Applied force to the cruciform specimen is carried through not only the gauge area but also other regions of the specimen. However, fraction of the force carried through gauge area is depend on specimen geometry and material constants, and unable to be determined simply. Then, stresses (σ x and σ y ) had to be calculated from elastic constants and the biaxial strains. In Fig. 7, ydirectional stress σ y is negative value, which means that gauge area is transversely compressed even though the specimen is subjected to uniaxial load. Biaxial strains under certain biaxial load ratios can be calculated based on the relationship between biaxial strains and uniaxial load with superposition principle in the y mal Stress x (a) xdirectional stress (Pa) mal Strain (b) xdirectional strain (m/m) E E y mal Stress x (c) ydirectional stress E+81.5E+8 (Pa) (m/m) Fig. 4. Calculated normal stress and strain in cruciform specimens under uniaxial loading (F x =100kN, F y =0kN). mal Strain (d) ydirectional strain
6 y mal Stress x (a) xdirectional stress (Pa) (m/m) Fig. 5. Calculated xdirectional normal stress and strain in cruciform specimens under uniaxial loading (F x =100kN, F y =100kN). range of linear elastic. As an example, several relationships among strain ratio, load ratio and stress ratio are shown in Table 3. In the table, stress is calculated by using strain and elastic constants in Table 1. These ratios are not necessarily coincident with each other with the exception of ratio 1:1 and 1:1. It is noted in the inplane biaxial tests with the cruciform specimens that load ratio has to be determined based on the relationships between load ratio and strain ratio in the gauge area. mal Strain (b) xdirectional strain Failure under Biaxial Loading Relationships between load and strain under biaxial load F x : F y =0.21:1 and 1:1 in the biaxial fracture tests are shown in Fig. 8. In Fig. 8(a), the cruciform specimen was subjected to biaxial load with load ratio F x : F y =0.21:1, and x and ydirectional strains increased as if stress state is uniaxial, which means ratio of xdirectional contraction to ydirectional extension is equal to Poisson s ratio. In Fig. 8(b), x and y directional strains increase accordance with applied load approximately equally due to the load ratio F x : F y =1:1. Inclination of the strain curves after the half of the fracture load are slightly changing in accordance with applied load, though strains at an early stage of the biaxial loading are almost proportional to the applied load. It is supposed that damages such as matrix cracks occurred at the later stage of the fracture tests and the degradation of stiffness due to the damages were the cause of the inclination change at the later stage of the fracture. Photographs of fracture near the gauge area of the cruciform specimen under biaxial loading F x : F y =1:1 were taken by a high speed camera (model:exilim EXF1, Casio Computer Co., Ltd., Japan) as shown in Fig. 9. The photographs were taken with frame rate 300 frame/second and resolution pixels. Figure 9 indicates that fracture was initiated at the gauge area, and subsequently breakage in GFRP tabs was developed in the directions of x and y axes. Photographs of the cruciform specimens after the biaxial fracture tests with load ratio F x : F y =0.21:1 and 1:1 are shown in Fig. 10. Breakage in the cruciform specimen with load control typically reaches the free edge of the cruciform specimens, especially
7 corner fillets. Figure 10 reveals that the breakage stops away from the free edges of the cruciform specimens, though the biaxial load was applied to the specimen with load control. In the experiments, the control system of the biaxial testing machine detects drastic load reduction, which means the stiffness reduction due to the fracture at the gauge area, and immediately activated an emergency stop with displacement control before the breakage reaches the free edges of the specimen. Fractures under ydirectional uniaxial stress at the gauge area was developed to x direction only as shown in Fig.10(a). Fractures under biaxial stress (σx=σy) was developed to both x and ydirections from the gauge area as shown in Fig. 10(b). Effect of Biaxial Loadings on Biaxial Strength Biaxial failure strain measured with using the cruciform specimens is shown in Fig. 11. In this figure, failure strain measured with using strip specimens under uniaxial loading is also plotted. The strip specimen size was 150mm length, 15mm width and 1mm thickness. Stacking sequence of the strip laminate was (45/0/45/90)s. Fracture strains obtained with the strip specimens were approximately equal to those obtained with the cruciform specimens in the uniaxial stress condition. The approximated correspondence of fracture strains under uniaxial stress in both strip and cruciform specimens indicates validity of inplane biaxial strength testing with cruciform specimens. Biaxial failure strains with strain ratios ε x : ε y =1:1, 0.3:1, 0.3:1, and 0.7:1 are plotted in Fig. 11. In the first quadrant of Fig. 11 (ε x : ε y =1:1, 0.3:1), ydirectional failure strains are approximately constant irrespective of xdirectional failure strain. In the second quadrant of Fig. 11(ε x : ε y =0.3:1, 0.7:1), ydirectional failure strains are also approximately constant irrespective of xdirectional failure strain. Comparing the first and second quadrants, ydirectional failure strains in the second quadrant are larger than those in the first quadrant. However, more data for biaxial strength is required to widen the range of failure envelope to all quadrants and to decrease sampling error due to the small samples. CONCLUSIONS The biaxial strength of quasiisotropic CFRP laminates was experimentally acquired with using the cruciform specimens. Strain and stress distributions in gauge area of the cruciform specimen were evaluated by finite element analysis and compared to validate measured strain level and ratio. Biaxial load ratio to obtain the final biaxial failure strains with prescribed strain ratio was calculated based on the relationships between biaxial load and strain under uniaxial loadings. High speed photographs of biaxial fracture indicated that failure was initiated at gauge area and breakage was developed to GFRP tab regions in the specimen. In the first quadrant of failure strain envelope, y directional failure stains were approximately constant irrespective of xdirectional failure strain. However, fracture strains in the second quadrant of the failure envelope were larger than those in the first quadrant. Failure strains under uniaxial stress measured with the cruciform specimens were compared with those measured with the strip specimens. Approximated accordance of fracture strains under uniaxial stress
8 irrespective of specimen type indicated validity of inplane biaxial strength tests with cruciform specimens. References 1. Hinton M.J., Kaddour A.S. and Soden P.D., Failure Criteria in Fibre Reinforced Polymer Composites: The WorldWide Failure Exercise, Elsevier Science Ltd, Oxford, UK, Mailly L. and Wang S.S., Recent Development of Planar Cruciform Experiment on Biaxial Tensile Deformation and Failure of Unidirectional Glass/Epoxy Composite, Journal of Composite Materials, Vol. 42, No. 13, pp , Smits A., Van Hemelrijcka D., Philippidisb T.P. and Cardona A., Design of a Cruciform Specimen for Biaxial Testing of Fibre Reinforced Composite Laminates, Composites Science and Technology, Vol. 66, No. 78, pp , Welsh J.S., Mayes J.S. and Biskne A.C., 2D Biaxial Testing and Failure Predictions of IM7/9772 Carbon/Epoxy QuasiIsotropic Laminates, Composite Structures, Vol. 75, No. 14, pp , Susuki I., Strength Properties of Composite Laminate under Biaxial Loadings, Proceedings of the Tenth International Conference on Composite Materials (ICCM10)  Volume IV: Characterization and Ceramic Matrix Composites, pp , Khamseh A.R. and Waas A. M., Failure Mechanisms of Composite Plates with a Circular Hole under Remote Biaxial Planar Compressive Loads, Journal of engineering materials and technology, Vol. 119, No. 1, pp , Strain (%) HTA/#101 (0/90/45/45)s #02 Fx : Fy = 1 : 0 ε x (experiment) ε y (experiment) ε x (FEM) ε y (FEM) Strain (%) HTA/#101 (0/90/45/45)s #06 Fx : Fy = 1 : 1 ε x (experiment) ε y (experiment) ε x (FEM) ε y (FEM) Load Fx(kN) Load Fy (kn) (a) F x : F y = 1 : 0 (b) F x : F y = 1 : 1 Fig. 6. Comparison between measured and calculated strains under biaxial load (F x : F y =1:0 and 1:1).
9 Strain (%) HTA/#101 (0/90/45/45)s #02 Fx : Fy = 1 : 0 ε x ε y σ x σ y Stress (MPa) Load Fx(kN) Fig. 7. Biaxial strain and stress under uniaxial load (F x : F y =1:0). Table 3. Ratio of biaxial strain, load and stress. strain ratio load ratio stress ratio εx:εy F x:f y σx:σy 1:1 1:1 1:1 0.3:1 0.68:1 0.56:10.3:1 0.21:1 0.01:10.7:10.34:10.5:11:11:11: HTA/#101 (0/90/45/45)s #15 Fx : Fy = 0.21 : 1 : ε X : ε Y HTA/#101 (0/90/45/45)s #17 Fx : Fy = 1 : 1 : ε X : ε Y Strain (%) 0.5 Strain (%) Load Fy (kn) Load Fy (kn) (a) F x : F y = 0.21 : 1 (b) F x : F y = 1 : 1 Fig. 8. Loadstrain curves under biaxial loading ratio F x : F y =1:1 and 0.21:1.
10 Fig.9. High Speed photograph of fracture in gauge area of cruciform specimen under biaxial loading (F x : F y =1:1). y x (a) F x : F y = 0.21 : 1 (b) F x : F y = 1 : 1 Fig.10. Fracture of cruciform specimens under biaxial loading (F x : F y = 0.21:1 and 1:1) 2 HTA/#101quasiisotropic : cruciform specimen : strip specimen ε Y (%) ε X (%) Fig. 11. Biaxial failure strain of CF/Epoxy quasiisotropic laminates.
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationEVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES
EVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES Koji YAMAGUCHI 1, Isao KIMPARA 1, and Kazuro KAGEYAMA 1 1 Department of Environmental &
More informationDIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE
DIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE Ab Ghani A. F Sustainable Maintenance Engineering Research Group, Universiti Teknikal Malaysia Melaka,
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationDEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS
DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8  PART 3 PROVISIONS Konstantinos CHRISTIDIS 1, Emmanouil VOUGIOUKAS 2 and Konstantinos TREZOS 3 ABSTRACT
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationBUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS
BUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS R. Degenhardt, H. Klein, A. Kling, H. Temmen, R. Zimmermann DLR Institute of Structural Mechanics Lilienthalplatz 7, 388
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationModeling the bond of GFRP and concrete based on a damage evolution approach
Modeling the ond of GFRP and concrete ased on a damage evolution approach Mohammadali Rezazadeh 1, Valter Carvelli 2, and Ana Veljkovic 3 1 Dep. Architecture, Built environment and Construction engineering,
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationASSESSMENT OF DYNAMICALLY LOADED CRACKS IN FILLETS
ASSESSMENT OF DNAMICALL LOADED CRACKS IN FILLETS Uwe Zencker, Linan Qiao, Bernhard Droste Federal Institute for Materials Research and Testing (BAM) 12200 Berlin, Germany email: zencker@web.de Abstract
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationITE IMPACT ON. Summary. concurrent. phenomena delamination. subroutine. simulations discussed. Keywords: Volnei Tita.
NUMERICAL AND EXPERIMENTAL ANALYSES OF LOW VELOCITY IMPACT ON THIN COMPOS ITE Marcelo L. Ribeiro Department of Aeronautical Engineeringg Engineering Scholl of São Carlos University of São S Paulo malribei@usp.
More informationA Critical Planeenergy Model for Multiaxial Fatigue Life Prediction. of Homogeneous and Heterogeneous Materials. Haoyang Wei
A Critical Planeenergy Model for Multiaxial Fatigue Life Prediction of Homogeneous and Heterogeneous Materials by Haoyang Wei A Thesis Presented in Partial Fulfillment of the Requirements for the Degree
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationLAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES. Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp.
LAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp. 12611266 INTRODUCTION Michael D. Seale and Barry T. Smith Departments
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More information